Active Standard ASTM F1869 | Developed by Subcommittee: F06.40
Book of Standards Volume: 15.04
Historical (view previous versions of standard)
Significance and Use
Use this test method to obtain a quantitative value indicating the rate of moisture vapor emission from the surface of a concrete floor and whether or not that floor is acceptable to receive resilient floor covering. The moisture vapor emission rate only reflects the condition of the concrete floor at the time of the test. All concrete subfloors emit some amount of moisture in vapor form. Concrete moisture emission is a natural process driven by environmental conditions. All floor coverings are susceptible to failure from excessive moisture vapor emissions. The moisture vapor emitted from a concrete slab is measured in pounds. This measurement is the equivalent weight of water evaporating from 1000 ft2 of concrete surface in a 24–h period. The calcium chloride moisture test has been the industry standard for making this determination and is a practical, well-established and accepted test of dynamic moisture. It will produce quantified results directly applicable to flooring manufacturer's specifications. The results obtained reflect the condition of the concrete floor surface at the time of testing and may not indicate future conditions.
1.1 This test method covers the quantitative determination of the rate of moisture vapor emitted from below-grade, on-grade, and above-grade (suspended) bare concrete floors.
1.2 This test shall not be used to evaluate the rate of moisture vapor emitted by lightweight or gypsum concrete floors containing lightweight aggregate.
1.3 This test shall not be used to evaluate moisture vapor emissions over coatings on concrete or through reactive penetrants or over patching or leveling compounds.
1.4 This quantity of moisture shall be expressed as the rate of moisture vapor emission, measured in pounds of moisture over a 1000 ft2 area during a 24-h period.
1.5 The values stated in inch-pound units are to be regarded as standard. The values given in parentheses are mathematical conversions to SI units that are provided for information only and are not considered standard.
1.6 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices, and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
Military StandardMIL-PRF-131 Barrier Materials, Waterproof, Greaseproof, Flexible, Heat-Sealable
E1745 Specification for Plastic Water Vapor Retarders Used in Contact with Soil or Granular Fill under Concrete Slabs
E1993 Specification for Bituminous Water Vapor Retarders Used in Contact with Soil or Granular Fill Under Concrete Slabs
F141 Terminology Relating to Resilient Floor Coverings
ICRI GuideICRITechnicalGuideli Selecting and Specifying Concrete Surface Preparation for Sealers, Coatings, and Polymer Overlays
Resilient Floor Covering Institute StandardRecommendedWorkPract
ICS Number Code 91.100.30 (Concrete and concrete products); 91.060.30 (Ceilings. Floors. Stairs)
UNSPSC Code 30161700(Flooring); 51182401(Calcium chloride)